LaAlO3 and SrTiO3 are insulating, non-magnetic oxides, yet the interface between them exhibits a two-dimensional electron system with high electron mobility1, superconductivity at low temperatures2,3,4,5,6 and electric-field-tuned metal–insulator and superconductor–insulator phase transitions3,6,7,8. Bulk magnetization and magnetoresistance measurements also indicate some form of magnetism depending on preparation conditions5,9,10,11 and a tendency towards nanoscale electronic phase separation10. Here we use local imaging of the magnetization and magnetic susceptibility to directly observe a landscape of ferromagnetism, paramagnetism and superconductivity. We find submicrometre patches of ferromagnetism in a uniform background of paramagnetism, with a non-uniform, weak diamagnetic superconducting susceptibility at low temperature. These results demonstrate the existence of nanoscale phase separation as indicated by theoretical predictions based on nearly degenerate interface sub-bands associated with the Ti orbitals12,13. The magnitude and temperature dependence of the paramagnetic response indicate that the vast majority of the electrons at the interface are localized14, and do not contribute to transport measurements3,6,7. In addition to the implications for magnetism, the existence of a two-dimensional superconductor at an interface with highly broken inversion symmetry and a ferromagnetic landscape in the background indicates the potential for exotic superconducting phenomena.
Coexistence of ferromagnetism and superconductivity in nature is rare15,16,17,18,19. The LaAlO3/SrTiO3 (LAO/STO) interface is a new system for studying this coexistence. LAO and STO are both perovskite band insulators with no magnetic order in their bulk form. For LAO grown on the TiO2-terminated STO substrate, a high-mobility electron gas was observed at the interface1. Electronic reconstruction, driven by the polar/nonpolar interface, is thought to move charge from the LAO layers across the interface into the STO, causing an effective electronic doping responsible for the observed conductivity1. The interplay of this effect with oxygen vacancies and structural changes20, and the relative contribution of these three effects to the carrier concentration, remains a subject of debate. Significant variability in the physical properties in similar samples indicates that the ground state of this interface system is sensitive to small changes in growth conditions. Superconductivity2,3,4,5 and features interpreted as interface magnetism5,9,10 have been independently observed at the LAO/STO interface through transport and bulk magnetization measurements. One recent study inferred the existence of both ferromagnetism and superconductivity in the same sample from hysteresis in magnetoresistance transport measurements5.
We use a scanning superconducting quantum interference device (SQUID) with micrometre-scale spatial resolution to image three samples down to 20 mK (see Methods). Our SQUID sensor can concurrently measure the static magnetic fields generated by the sample (magnetometry) and the susceptibility of the sample to a small locally applied a.c. magnetic field (susceptometry). Figure 1a,c shows magnetometry and susceptometry images of an LAO/STO interface. The ferromagnetic landscape appears as many static spatially separated dipoles that show no temperature dependence over the measured temperature range. The superconductivity is spatially inhomogeneous and weak, with a critical temperature Tc=100 mK (Fig. 1e), above which a temperature-dependent paramagnetic response is apparent (Fig. 1e inset). In contrast, a δ-doped STO sample21 has relatively uniform two-dimensional superconductivity, no magnetic order and no apparent paramagnetic response above Tc (Fig. 1b,d,f), although the expected paramagnetic signal at Tc=300 mK is close to our noise floor.
The diamagnetic susceptibility from the LAO/STO interface is an order of magnitude smaller than that of the δ-doped SrTiO3 or (Ba0.9Nb0.1CuO2+x)m/(CaCuO2)n, another two-dimensional superconductor22. The susceptometry signal is generated by superconducting electrons that screen the local applied field and is related to the local density of electrons in the superconducting condensate. The superfluid density is usually quantified by the magnetic penetration depth, λ (refs 23, 24). In a two-dimensional superconductor with thickness d≪λ, the screening currents are confined in the vertical direction, which generates a modified penetration depth known as the Pearl length, Λ=2λ2/d. The low-temperature Pearl length in the δ-doped STO sample was 650 μm on the basis of fits to formulas for the height dependence of the susceptometry from refs 24, 25. This formula should not quantitatively describe the data for the LAO/STO interface owing to the lateral inhomogeneities, but the susceptibility signal from a uniform two-dimensional superconductor scales as 1/Λ for large Λ, implying an ∼8 mm Pearl length in the LAO/STO.
The Tc variation between two measurement positions on the LAO/STO sample (Fig. 1e) is about 10%. However, the lateral variation of the susceptometry is large: 84% of the total response, compared with just 12% in the δ-doped STO, and less than 1% in most bulk superconductors26. The largely inhomogeneous superconducting and ferromagnetic response may indicate proximity to a first-order phase transition. Although both magnetism and superconductivity are present at the interface in the LAO/STO sample, Fig. 1a,c does not show a direct correlation between the inhomogeneity of the superconducting state and the distribution of magnetic regions.
The ferromagnetism appears as magnetic dipoles in Figs 1a and 2a, mostly separated from one another by micrometres, with many extra dipoles that do not show up visually in these images but are still above our noise threshold (Fig. 2a insets). We analysed six 70×80 μm high-resolution magnetometry scans, including the one shown in Fig. 2a, finding 144 dipoles above our noise floor and fitting each one to a point-dipole model to determine its total moment and orientation (Fig. 2b–d). The histogram of the dipole moments shows a clear exponential distribution of dipole moments with a few large (∼1×108 μB) dipoles and substantially more smaller dipoles down to the limit of our noise. This trend indicates that there may be even more dipoles with moments below the sensitivity of our SQUID.
Most of the dipoles lie in plane, as expected from the shape anisotropy of the interface, with apparently randomly distributed azimuthal angles indicating no alignment or net magnetization. This observation is consistent with cooling the sample in zero field. The point-dipole approximation is not as good for some dipoles, particularly the ones with the largest moments, indicating that they are not point-like but are instead ferromagnetic patches that extend over an area comparable to the SQUID’s 3 μm pick-up loop. The dipoles were stable throughout the duration of the cool-down (about 1 month) and were insensitive to temperature changes from 20 mK through the superconducting critical temperature and up to 4.2 K. Further SQUID measurements in a separate variable-temperature cryostat showed that the dipole size and orientation remained unchanged between 4.2 K and our maximum measurement temperature of 60 K. In addition, we measured a second sample with 10 unit cells (u.c.) of LAO grown on a TiO2-terminated surface that had patterned Hall bars (Methods). This second 10 u.c. LAO/STO sample had many fewer dipoles—none in some regions. The variability in the size of the moment may be related to the variability of physical properties in nominally identical samples in this system.
We did not observe dipoles in the magnetometry signal on the δ-doped STO sample (Fig. 1b). As both the δ-doped STO sample and the LAO/STO samples use the same commercially available STO substrates, the absence of dipoles on the δ-doped STO sample rules out magnetic impurities in the substrate. This observation is corroborated by the scan height extracted from the dipole fits, indicating that the dipoles are within a few micrometres of the surface.
In addition to the ferromagnetic order, the two LAO/STO samples measured at low temperature show paramagnetism above the superconducting critical temperature Tc (Fig. 1e inset, Fig. 3). In the case of the patterned LAO/STO sample, which did not show many ferromagnetic dipoles, we observed regions near the Hall-bar edges where the superconductivity was suppressed and the paramagnetism remained down to the lowest measured temperatures. The paramagnetic signal decreases with increasing temperature, indicating a Curie law. The 1/T dependence and the paramagnetic sign indicate that the susceptibility signal originates from localized spins.
We can estimate the electron density associated with the ferromagnetic, diamagnetic and paramagnetic signals. We determine the number of ferromagnetic electrons by adding the moments of all the dipoles in the histogram, yielding 7.3±3.4×1012 μB cm−2. This estimate is a lower bound, because any dipoles that are below the sensitivity of our sensor or whose moments cancelled owing to the random distribution of alignments have not been included in this total. We use the Pearl length to find the density of superconducting electrons, ns=2m*/μ0e2Λ, where eis the elementary charge and μ0 is the permeability of free space. Using m*=1.45 me(ref. 27), we find ns≈1×1012 cm−2 in the regions of high superfluid density and ns≈3×1011 cm−2 in the regions of low superfluid density. We quantify the paramagnetic signal by using an appropriate model for our sensor to convert our measured susceptibility, ϕ, to the dimensionless susceptibility, χ, for a layer of spins in a thickness d. Using χ d=22 μm(mA/Φ0)ϕ (ref. 28) and comparing χwith the Curie expression, χ=μ0n3D(g μB)2J(J+1)/3kBT with g=2 and J=1/2, yields a two-dimensional spin density of 4.4×1014 cm−2, with large error bars due to uncertainty in the geometrical parameters. We compare our estimates with the electron densities predicted by the polar catastrophe, 3×1014 cm−2, and seen in Hall measurements3,6,7, 1–4×1013 cm−2 (Table 1). The densities of magnetic and superconducting electrons are respectively one and two orders of magnitude lower than the polar catastrophe density, but the paramagnetic spin density shows surprising agreement within error.
Density functional calculations of the electronic structure in LAO/STO predict the presence of multiple nearly degenerate subbands that result in separate charge carriers12. Magnetism was also predicted at the n-type LAO/STO interface from alignment of extra electrons in the Ti orbitals13. Transport measurements, which probe delocalized electrons, have measured electron densities significantly lower than predictions from the polar catastrophe. Our measurements indicate that these missing electrons may be present but localized, and contribute to the magnetic signal.
The observation of ferromagnetism and superconductivity at the LAO/STO interface opens exciting possibilities for studying the interplay of these normally incompatible states. Tuning the carriers with a gate voltage may add even more richness to the system, by coincidentally studying how adding or removing carriers affects the superconducting, ferromagnetic and paramagnetic signals.
Note added in proof: Recent torque magnetometry in a similar sample29 shows magnetic ordering consistent with interface magnetism. The variety of details in reports of magnetism9,10,11,29, including our observation of a landscape (rather than a homogeneous phase), support the exciting possibility that multiple states are important in this engineered interface.
The two LAO/STO samples used in the low-temperature study were prepared by growing 10 u.c. of LaAlO3 on commercial TiO2-terminated 001 STO substrates. The patterned sample had an AlOx hard mask, which defined Hall bars. The LaAlO3 was deposited at 800 °C with an oxygen partial pressure of 10−5 mbar, after a pre-anneal at 950 °C with an oxygen partial pressure of 5×10−6 mbar for 30 min. The samples were cooled to 600 °C and annealed in a high-pressure oxygen environment (0.4 bar) for one hour6.
A δ-doped STO sample was also studied at low temperatures. It was grown in an atmosphere of less than 10−8 torr oxygen at 1,200 °C. Nb dopants were confined to a 5.9 nm layer, and further 100 nm cap and buffer layers of STO were grown above and below the doped region. The sample was annealed in situ at 900 °C under an oxygen partial pressure of 10−2 torr for 30 min (ref. 21).
Measurements were made by scanning SQUID in a dilution refrigerator30,31. The SQUID has a 3 μm pick-up loop, centred in a single-turn field coil. Static magnetism (magnetometry) in the sample is probed by recording the flux through the SQUID pick-up loop as a function of position. Applying an a.c. current in the field coil produces a local magnetic field. The local susceptibility (susceptometry) of the sample to the applied field is detected by the pick-up loop in a lock-in measurement.
Ohtomo, A. & Hwang, H. Y. A high-mobility electron gas at the LaAlO3/SrTiO3 heterointerface. Nature 427, 423–426 (2004).
Reyren, N. et al. Superconducting interfaces between insulating oxides. Science 317, 1196–1199 (2007).
Caviglia, A. D. et al. Electric field control of the LaAlO3/SrTiO3 interface ground state. Nature 456, 624–627 (2008).
Ben Shalom, M., Sachs, M., Rakhmilevitch, D., Palevski, A. & Dagan, Y. Tuning spin–orbit coupling and superconductivity at the SrTiO3/LaAlO3 interface: A magnetotransport study. Phys. Rev. Lett. 104, 126802 (2010).
Dikin, D. A. et al. Coexistence of superconductivity and ferromagnetism in two dimensions. Phys. Rev. Lett. 107, 056802 (2011).
Bell, C. et al. Dominant mobility modulation by the electric field effect at the LaAlO3/SrTiO3 interface. Phys. Rev. Lett. 103, 226802 (2009).
Thiel, S., Hammerl, G., Schmehl, A., Schneider, C. W. & Mannhart, J. Tunable quasi-two-dimensional electron gases in oxide heterostructures. Science 313, 1942–1945 (2006).
Cen, C. et al. Nanoscale control of an interfacial metal–insulator transition at room temperature. Nature Mater. 7, 298–302 (2008).
Brinkman, A. et al. Magnetic effects at the interface between non-magnetic oxides. Nature Mater. 6, 493–496 (2007).
Ariando, et al. Electronic phase separation at the LaAlO3/SrTiO3 interface. Nature Commun. 2, 188 (2011).
Seri, S. & Klein, L. Antisymmetric magnetoresistance of the SrTiO3/LaAlO3 interface. Phys. Rev. B 80, 180410 (2009).
Popović, Z. S., Satpathy, S. & Martin, R. M. Origin of the two-dimensional electron gas carrier density at the LaAlO3 on SrTiO3 interface. Phys. Rev. Lett. 101, 256801 (2008).
Pentcheva, R. & Pickett, W. E. Charge localization or itineracy at LaAlO3/SrTiO3 interfaces: Hole polarons, oxygen vacancies, and mobile electrons. Phys. Rev. B 74, 035112 (2006).
Sing, M. et al. Profiling the interface electron gas of LaAlO3/SrTiO3 heterostructures with hard X-ray photoelectron spectroscopy. Phys. Rev. Lett. 102, 176805 (2009).
Aoki, D. et al. Coexistence of superconductivity and ferromagnetism in URhGe. Nature 413, 613–616 (2001).
Saxena, S. S. et al. Superconductivity on the border of itinerant-electron ferromagnetism in UGe2 . Nature 406, 587–592 (2000).
Bulaevskii, L. N., Buzdin, A. I., Kulic, M. L. & Panjukov, S. V. Coexistence of superconductivity and magnetism. Theoretical predictions and experimental results. Adv. Phys. 34, 175–261 (1985).
Buzdin, A. I. Proximity effects in superconductor–ferromagnet heterostructures. Rev. Mod. Phys. 77, 935–976 (2005).
Tallon, J. et al. Coexisting ferromagnetism and superconductivity in hybrid rutheno-cuprate superconductors. Appl. Supercond. 9, 1696–1699 (1999).
Huijben, M. et al. Structure property relation of SrTiO3/LaAlO3 interfaces. Adv. Mater. 21, 1665–1677 (2009).
Kozuka, Y. et al. Two-dimensional normal-state quantum oscillations in a superconducting heterostructure. Nature 462, 487–490 (2009).
Tafuri, F., Kirtley, J. R., Medaglia, P. G., Orgiani, P. & Balestrino, G. Magnetic imaging of Pearl vortices in artificially layered (Ba0.9Nd0.1CuO2+x)m/(CaCuO2)n systems. Phys. Rev. Lett. 92, 157006 (2004).
Luan, L. et al. Local measurement of the penetration depth in the pnictide superconductor Ba(Fe0.95Co0.05)2As2 . Phys. Rev. B 81, 100501 (2010).
Hicks, C. W. et al. Evidence for a nodal energy gap in the iron-pnictide superconductor LaFePO from penetration depth measurements by scanning SQUID susceptometry. Phys. Rev. Lett. 103, 127003 (2009).
Kogan, V. G. Meissner response of anisotropic superconductors. Phys. Rev. B 68, 104511 (2003).
Kalisky, B. et al. Stripes of increased diamagnetic susceptibility in underdoped superconducting Ba(Fe1−xCox)2As2 single crystals: Evidence for an enhanced superfluid density at twin boundaries. Phys. Rev. B 81, 184513 (2010).
Caviglia, A. D. et al. Two-dimensional quantum oscillations of the conductance at LaAlO3/SrTiO3 interfaces. Phys. Rev. Lett. 105, 236802 (2010).
Bluhm, H., Bert, J. A., Koshnick, N. C., Huber, M. E. & Moler, K. A. Spinlike susceptibility of metallic and insulating thin films at low temperature. Phys. Rev. Lett. 103, 026805 (2009).
Li, L., Richter, C., Mannhart, J. & Ashoori, R. C. Coexistence of magnetic order and two-dimensional superconductivity at LaAlO3/SrTiO3 interfaces. Nature Phys. 7,http://dx.doi.org/10.1038/nphys2080 (2011).
Huber, M. E. et al. Gradiometric micro-SQUID susceptometer for scanning measurements of mesoscopic samples. Rev. Sci. Instrum. 79, 053704 (2008).
Björnsson, P. G., Gardner, B. W., Kirtley, J. R. & Moler, K. A. Scanning superconducting quantum interference device microscope in a dilution refrigerator. Rev. Sci. Instrum. 72, 4153–4158 (2001).
We thank M. Huber for assistance in SQUID design and fabrication. This work was primarily supported by the US Department of Energy, Office of Basic Energy Sciences, Division of Materials Sciences and Engineering under award DE-AC02-76SF00515. B.K. acknowledges support from FENA.
The authors declare no competing financial interests.
About this article
Cite this article
Bert, J., Kalisky, B., Bell, C. et al. Direct imaging of the coexistence of ferromagnetism and superconductivity at the LaAlO3/SrTiO3 interface. Nature Phys 7, 767–771 (2011). https://doi.org/10.1038/nphys2079
This article is cited by
Nature Physics (2023)
npj Quantum Materials (2022)
Emergence of electric-field-tunable interfacial ferromagnetism in 2D antiferromagnet heterostructures
Nature Communications (2022)
Nature Physics (2022)
npj Quantum Materials (2022)